# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.
# This journal is © The Royal Society of Chemistry 2017

 
data_shelx
 
_audit_creation_method            'SHELXL-97'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          
 'O32 P9 V4, 7(Na)'
_chemical_formula_sum
 'Na7 O32 P9 V4' 
_chemical_formula_weight          1155.42

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'V'  'V'   0.3005   0.5294
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       tetragonal
_space_group_IT_number            114
_space_group_name_H-M_alt         'P -4 21 c'
_space_group_name_Hall            'P -4 2n'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 'x+1/2, -y+1/2, -z+1/2'
 '-x, -y, z'
 '-x+1/2, y+1/2, -z+1/2'
 '-y+1/2, -x+1/2, z+1/2'
 '-y, x, -z'
 'y, -x, -z'
 'y+1/2, x+1/2, z+1/2'
 
_cell_length_a                    14.212(5)
_cell_length_b                    14.212
_cell_length_c                    6.337(2)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      1279.9(9)
_cell_formula_units_Z             2
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     6974
_cell_measurement_theta_min       2.87
_cell_measurement_theta_max       30.56
 
_exptl_crystal_description        'needle' 
_exptl_crystal_colour             'yellow'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     2.998          
_exptl_crystal_F_000              1120
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.16
_exptl_crystal_size_mid           0.08
_exptl_crystal_size_min           0.07 
_exptl_absorpt_coefficient_mu     2.241
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.6653
_exptl_absorpt_correction_T_max   0.7461
_exptl_absorpt_process_details    'Bruker SADABS' 
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'fine-focus sealed tube'  
_diffrn_measurement_device_type   'PHOTON 100 CMOS'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             17162
_diffrn_reflns_av_unetI/netI      0.0437
_diffrn_reflns_av_R_equivalents   0.0775
_diffrn_reflns_limit_h_min        -20
_diffrn_reflns_limit_h_max        20
_diffrn_reflns_limit_k_min        -20
_diffrn_reflns_limit_k_max        19
_diffrn_reflns_limit_l_min        -9
_diffrn_reflns_limit_l_max        9
_diffrn_reflns_theta_min          2.867
_diffrn_reflns_theta_max          30.679
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.990
_diffrn_measured_fraction_theta_full  0.997
_diffrn_reflns_Laue_measured_fraction_max    0.990
_diffrn_reflns_Laue_measured_fraction_full   0.997
_diffrn_reflns_point_group_measured_fraction_max   0.990
_diffrn_reflns_point_group_measured_fraction_full  0.998
_reflns_number_total              1963
_reflns_number_gt                 1722
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.732
_reflns_Friedel_fraction_max      0.990
_reflns_Friedel_fraction_full     1.000
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'Bruker APEX3'
_computing_cell_refinement        'Bruker SAINT'
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'Superflip (Palatinus & Chapuis, 2007)'
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 97)'
_computing_molecular_graphics     'ATOMS (Dowty, 2002)'
_computing_publication_material   ?
_refine_special_details
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0262P)²+0.8673P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack    0.43(4)
_chemical_absolute_configuration  ?
_refine_ls_number_reflns          1963
_refine_ls_number_parameters      119
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0438
_refine_ls_R_factor_gt            0.0326
_refine_ls_wR_factor_ref          0.0620
_refine_ls_wR_factor_gt           0.0590
_refine_ls_goodness_of_fit_ref    1.038
_refine_ls_restrained_S_all       1.038
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
V1 V 0.81624(4) 0.12034(4) 0.12976(11) 0.00596(14) Uani 1 1 d . . . . .
P1 P 0.0000 0.0000 0.0000 0.0057(4) Uani 1 4 d S T P . .
P2 P 0.61985(7) 0.25690(7) 0.14137(15) 0.00642(19) Uani 1 1 d . . . . .
P3 P 0.95619(7) 0.30282(7) 0.11002(17) 0.00721(19) Uani 1 1 d . . . . .
Na1 Na 0.0000 0.0000 0.5000 0.0619(16) Uani 1 4 d S T P . .
Na2 Na 0.0000 0.5000 0.8278(4) 0.0287(7) Uani 1 2 d S T P . .
Na3 Na 0.91816(13) 0.25935(13) 0.6041(3) 0.0200(4) Uani 1 1 d . . . . .
O1 O 0.13703(19) 0.17101(19) 0.1884(4) 0.0104(6) Uani 1 1 d . . . . .
O2 O 0.6995(2) 0.1912(2) 0.1025(5) 0.0177(6) Uani 1 1 d . . . . .
O3 O 0.93538(18) 0.05554(19) 0.1477(4) 0.0104(6) Uani 1 1 d . . . . .
O4 O 0.5359(2) 0.1880(2) 0.2107(5) 0.0151(6) Uani 1 1 d . . . . .
O5 O 0.5864(2) 0.3048(2) 0.9432(4) 0.0149(7) Uani 1 1 d . . . . .
O6 O 0.0020(2) 0.2570(2) 0.9201(4) 0.0115(6) Uani 1 1 d . . . . .
O7 O 0.9269(2) 0.40252(19) 0.0722(5) 0.0138(6) Uani 1 1 d . . . . .
O8 O 0.8796(2) 0.2434(2) 0.2074(5) 0.0173(7) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
V1 O3 1.931(3) . ?
V1 O2 1.949(3) . ?
V1 O6 2.003(3) 6_656 ?
V1 O8 2.027(3) . ?
V1 O1 2.039(3) 6_655 ?
V1 O5 2.051(3) 8_544 ?
V1 O4 3.437(3) 8_544 ?
V1 Na3 3.501(2) 6_646 ?
V1 O6 3.537(3) 1_654 ?
V1 O3 3.650(3) 6_645 ?
V1 O2 3.660(3) 8_545 ?
P1 O3 1.531(3) 6_545 ?
P1 O3 1.531(3) 3_655 ?
P1 O3 1.531(3) 7_565 ?
P1 O3 1.531(3) 1_455 ?
P1 Na1 3.1687(10) 1_554 ?
P1 Na1 3.1687(10) . ?
P1 O1 3.335(3) 3 ?
P1 O1 3.335(3) 6 ?
P1 O1 3.335(3) 7 ?
P1 O1 3.335(3) . ?
P2 O2 1.488(3) . ?
P2 O5 1.505(3) 1_554 ?
P2 O1 1.507(3) 2 ?
P2 O4 1.605(3) . ?
P2 Na3 3.040(2) 8_544 ?
P2 O2 3.199(3) 8_545 ?
P2 O6 3.251(3) 2_556 ?
P2 Na3 3.269(2) 2_455 ?
P2 O8 3.546(3) 2_455 ?
P3 O7 1.496(3) . ?
P3 O8 1.510(3) . ?
P3 O6 1.516(3) 1_654 ?
P3 O4 1.609(3) 2 ?
P3 Na2 3.1851(15) 5_654 ?
P3 O1 3.219(3) 1_655 ?
P3 Na3 3.237(2) . ?
P3 Na3 3.243(2) 8_544 ?
P3 Na3 3.309(2) 1_554 ?
P3 Na2 3.3822(17) 1_654 ?
P3 O7 3.503(3) 8_545 ?
P3 O1 3.521(3) 6_655 ?
Na1 O3 2.540(3) 7_566 ?
Na1 O3 2.540(3) 1_455 ?
Na1 O3 2.540(3) 3_655 ?
Na1 O3 2.540(3) 6_546 ?
Na1 O5 3.055(3) 2_456 ?
Na1 O5 3.055(3) 4_546 ?
Na1 O5 3.055(3) 8_444 ?
Na1 O5 3.055(3) 5_554 ?
Na1 P1 3.1687(10) 1_556 ?
Na1 O1 3.687(3) 3 ?
Na1 O1 3.687(3) 7_556 ?
Na2 O7 2.323(3) 3_666 ?
Na2 O7 2.323(3) 1_456 ?
Na2 O7 2.371(3) 8_445 ?
Na2 O7 2.371(3) 5_565 ?
Na2 O4 2.731(3) 6_556 ?
Na2 O4 2.731(3) 7_566 ?
Na2 Na2 3.1686(10) 5 ?
Na2 Na2 3.1687(11) 5_554 ?
Na2 P3 3.1851(17) 8_445 ?
Na2 P3 3.1851(17) 5_565 ?
Na2 P3 3.3822(17) 3_666 ?
Na2 P3 3.3822(17) 1_456 ?
Na3 O6 2.330(3) 1_655 ?
Na3 O7 2.400(3) 8_545 ?
Na3 O1 2.521(3) 6_656 ?
Na3 O5 2.577(4) 2_556 ?
Na3 O8 2.583(4) . ?
Na3 O4 2.709(4) 2 ?
Na3 P2 3.040(2) 8_545 ?
Na3 O8 3.086(4) 8_545 ?
Na3 O5 3.111(4) 8_544 ?
Na3 P3 3.243(2) 8_545 ?
Na3 P2 3.269(2) 2 ?
O1 P2 1.507(3) 2_455 ?
O1 V1 2.039(3) 7_565 ?
O1 O5 2.467(4) 2_456 ?
O1 Na3 2.521(3) 7_566 ?
O1 O2 2.525(4) 2_455 ?
O1 O4 2.547(4) 2_455 ?
O1 O2 2.717(4) 7_565 ?
O1 O6 2.840(4) 1_554 ?
O1 O3 2.857(4) 7_565 ?
O1 O8 3.016(4) 7_565 ?
O1 O6 3.070(4) 7_556 ?
O1 P3 3.219(3) 1_455 ?
O2 O4 2.424(4) . ?
O2 O5 2.491(4) 1_554 ?
O2 O1 2.525(4) 2 ?
O2 O1 2.717(4) 6_655 ?
O2 O8 2.747(4) . ?
O2 O6 2.762(4) 6_656 ?
O2 O5 3.020(4) 8_544 ?
O2 O2 3.1730(11) 8_545 ?
O2 O2 3.1730(11) 8_544 ?
O2 P2 3.199(3) 8_544 ?
O3 P1 1.531(3) 1_655 ?
O3 O3 2.422(5) 3_755 ?
O3 O3 2.537(5) 6_645 ?
O3 O3 2.537(5) 7_665 ?
O3 Na1 2.540(3) 1_655 ?
O3 O5 2.673(4) 8_544 ?
O3 O8 2.810(4) . ?
O3 O1 2.857(4) 6_655 ?
O3 O6 2.870(4) 6_656 ?
O3 O1 3.312(4) 1_655 ?
O3 O6 3.343(4) 1_654 ?
O4 P3 1.609(3) 2_455 ?
O4 O7 2.439(4) 2_455 ?
O4 O5 2.479(4) 1_554 ?
O4 O8 2.481(4) 2_455 ?
O4 O6 2.513(4) 2_556 ?
O4 O1 2.547(4) 2 ?
O4 Na3 2.709(4) 2_455 ?
O4 Na2 2.731(3) 6_656 ?
O4 O7 3.078(4) 7_565 ?
O4 O2 3.326(4) 8_545 ?
O5 P2 1.505(3) 1_556 ?
O5 V1 2.051(3) 8_545 ?
O5 O1 2.467(4) 2_556 ?
O5 O4 2.479(4) 1_556 ?
O5 O2 2.491(4) 1_556 ?
O5 Na3 2.577(4) 2_456 ?
O5 O3 2.673(4) 8_545 ?
O5 O6 2.740(4) 2_556 ?
O5 O8 2.887(4) 8_545 ?
O5 O2 3.020(4) 8_545 ?
O5 Na1 3.055(3) 2_556 ?
O5 Na3 3.111(4) 8_545 ?
O6 P3 1.516(3) 1_456 ?
O6 V1 2.003(3) 7_566 ?
O6 Na3 2.330(3) 1_455 ?
O6 O4 2.513(4) 2_456 ?
O6 O7 2.519(4) 1_456 ?
O6 O8 2.526(4) 1_456 ?
O6 O5 2.740(4) 2_456 ?
O6 O2 2.762(4) 7_566 ?
O6 O1 2.840(4) 1_556 ?
O6 O3 2.870(4) 7_566 ?
O6 O1 3.070(4) 6_556 ?
O6 P2 3.251(3) 2_456 ?
O7 Na2 2.323(3) 1_654 ?
O7 Na2 2.371(3) 5_654 ?
O7 Na3 2.400(3) 8_544 ?
O7 O4 2.439(4) 2 ?
O7 O8 2.511(4) . ?
O7 O6 2.519(4) 1_654 ?
O7 O4 3.078(4) 6_655 ?
O7 O7 3.2063(13) 8_545 ?
O7 O7 3.2063(14) 8_544 ?
O7 O7 3.463(6) 3_765 ?
O7 O8 3.500(4) 8_544 ?
O8 O4 2.481(5) 2 ?
O8 O6 2.526(4) 1_654 ?
O8 O5 2.887(4) 8_544 ?
O8 O1 3.016(4) 6_655 ?
O8 Na3 3.086(4) 8_544 ?
O8 O7 3.500(4) 8_545 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O3 V1 O2 176.81(13) . . ?
O3 V1 O6 93.70(11) . 6_656 ?
O2 V1 O6 88.69(12) . 6_656 ?
O3 V1 O8 90.43(13) . . ?
O2 V1 O8 87.38(13) . . ?
O6 V1 O8 173.35(12) 6_656 . ?
O3 V1 O1 92.05(12) . 6_655 ?
O2 V1 O1 85.87(13) . 6_655 ?
O6 V1 O1 89.30(11) 6_656 6_655 ?
O8 V1 O1 95.76(12) . 6_655 ?
O3 V1 O5 84.29(12) . 8_544 ?
O2 V1 O5 98.03(13) . 8_544 ?
O6 V1 O5 85.07(12) 6_656 8_544 ?
O8 V1 O5 90.16(13) . 8_544 ?
O1 V1 O5 173.07(12) 6_655 8_544 ?
O3 V1 O4 110.11(10) . 8_544 ?
O2 V1 O4 70.15(11) . 8_544 ?
O6 V1 O4 46.32(9) 6_656 8_544 ?
O8 V1 O4 136.41(11) . 8_544 ?
O1 V1 O4 47.43(9) 6_655 8_544 ?
O5 V1 O4 128.63(10) 8_544 8_544 ?
O3 V1 Na3 81.33(9) . 6_646 ?
O2 V1 Na3 101.85(10) . 6_646 ?
O6 V1 Na3 39.40(8) 6_656 6_646 ?
O8 V1 Na3 136.65(10) . 6_646 ?
O1 V1 Na3 126.82(9) 6_655 6_646 ?
O5 V1 Na3 46.84(9) 8_544 6_646 ?
O4 V1 Na3 85.58(6) 8_544 6_646 ?
O3 V1 O6 68.24(10) . 1_654 ?
O2 V1 O6 108.59(10) . 1_654 ?
O6 V1 O6 142.17(9) 6_656 1_654 ?
O8 V1 O6 44.44(9) . 1_654 ?
O1 V1 O6 59.87(9) 6_655 1_654 ?
O5 V1 O6 123.53(10) 8_544 1_654 ?
O4 V1 O6 107.29(7) 8_544 1_654 ?
Na3 V1 O6 149.41(6) 6_646 1_654 ?
O3 V1 O3 41.15(12) . 6_645 ?
O2 V1 O3 138.98(10) . 6_645 ?
O6 V1 O3 65.09(10) 6_656 6_645 ?
O8 V1 O3 121.08(10) . 6_645 ?
O1 V1 O3 64.07(9) 6_655 6_645 ?
O5 V1 O3 109.70(10) 8_544 6_645 ?
O4 V1 O3 68.96(7) 8_544 6_645 ?
Na3 V1 O3 78.12(5) 6_646 6_645 ?
O6 V1 O3 80.89(6) 1_654 6_645 ?
O3 V1 O2 121.61(10) . 8_545 ?
O2 V1 O2 60.03(7) . 8_545 ?
O6 V1 O2 97.74(10) 6_656 8_545 ?
O8 V1 O2 75.64(10) . 8_545 ?
O1 V1 O2 144.80(10) 6_655 8_545 ?
O5 V1 O2 40.60(10) 8_544 8_545 ?
O4 V1 O2 118.83(8) 8_544 8_545 ?
Na3 V1 O2 73.07(6) 6_646 8_545 ?
O6 V1 O2 120.09(7) 1_654 8_545 ?
O3 V1 O2 149.08(7) 6_645 8_545 ?
O3 P1 O3 111.96(11) 6_545 3_655 ?
O3 P1 O3 104.6(2) 6_545 7_565 ?
O3 P1 O3 111.96(11) 3_655 7_565 ?
O3 P1 O3 111.96(11) 6_545 1_455 ?
O3 P1 O3 104.6(2) 3_655 1_455 ?
O3 P1 O3 111.96(11) 7_565 1_455 ?
O3 P1 Na1 52.30(10) 6_545 1_554 ?
O3 P1 Na1 127.70(10) 3_655 1_554 ?
O3 P1 Na1 52.30(10) 7_565 1_554 ?
O3 P1 Na1 127.70(10) 1_455 1_554 ?
O3 P1 Na1 127.70(10) 6_545 . ?
O3 P1 Na1 52.30(10) 3_655 . ?
O3 P1 Na1 127.70(10) 7_565 . ?
O3 P1 Na1 52.30(10) 1_455 . ?
Na1 P1 Na1 180.0 1_554 . ?
O3 P1 O1 58.71(11) 6_545 3 ?
O3 P1 O1 75.85(11) 3_655 3 ?
O3 P1 O1 163.19(11) 7_565 3 ?
O3 P1 O1 78.84(11) 1_455 3 ?
Na1 P1 O1 110.98(5) 1_554 3 ?
Na1 P1 O1 69.02(5) . 3 ?
O3 P1 O1 75.85(11) 6_545 6 ?
O3 P1 O1 163.19(11) 3_655 6 ?
O3 P1 O1 78.84(11) 7_565 6 ?
O3 P1 O1 58.71(11) 1_455 6 ?
Na1 P1 O1 69.02(5) 1_554 6 ?
Na1 P1 O1 110.98(5) . 6 ?
O1 P1 O1 97.37(4) 3 6 ?
O3 P1 O1 78.84(11) 6_545 7 ?
O3 P1 O1 58.71(11) 3_655 7 ?
O3 P1 O1 75.85(11) 7_565 7 ?
O3 P1 O1 163.19(11) 1_455 7 ?
Na1 P1 O1 69.02(5) 1_554 7 ?
Na1 P1 O1 110.98(5) . 7 ?
O1 P1 O1 97.37(3) 3 7 ?
O1 P1 O1 138.04(9) 6 7 ?
O3 P1 O1 163.19(11) 6_545 . ?
O3 P1 O1 78.84(11) 3_655 . ?
O3 P1 O1 58.71(11) 7_565 . ?
O3 P1 O1 75.85(11) 1_455 . ?
Na1 P1 O1 110.98(5) 1_554 . ?
Na1 P1 O1 69.02(5) . . ?
O1 P1 O1 138.04(9) 3 . ?
O1 P1 O1 97.37(3) 6 . ?
O1 P1 O1 97.37(4) 7 . ?
O2 P2 O5 112.68(18) . 1_554 ?
O2 P2 O1 114.96(17) . 2 ?
O5 P2 O1 109.92(16) 1_554 2 ?
O2 P2 O4 103.17(18) . . ?
O5 P2 O4 105.65(18) 1_554 . ?
O1 P2 O4 109.82(16) 2 . ?
O2 P2 Na3 87.96(13) . 8_544 ?
O5 P2 Na3 78.47(13) 1_554 8_544 ?
O1 P2 Na3 55.77(12) 2 8_544 ?
O4 P2 Na3 165.07(12) . 8_544 ?
O2 P2 O2 75.52(11) . 8_545 ?
O5 P2 O2 167.82(14) 1_554 8_545 ?
O1 P2 O2 57.90(12) 2 8_545 ?
O4 P2 O2 80.20(13) . 8_545 ?
Na3 P2 O2 93.25(7) 8_544 8_545 ?
O2 P2 O6 119.68(14) . 2_556 ?
O5 P2 O6 125.33(14) 1_554 2_556 ?
O1 P2 O6 60.86(12) 2 2_556 ?
O4 P2 O6 49.14(12) . 2_556 ?
Na3 P2 O6 116.63(7) 8_544 2_556 ?
O2 P2 O6 50.71(8) 8_545 2_556 ?
O2 P2 Na3 122.93(13) . 2_455 ?
O5 P2 Na3 50.08(13) 1_554 2_455 ?
O1 P2 Na3 122.04(12) 2 2_455 ?
O4 P2 Na3 55.63(13) . 2_455 ?
Na3 P2 Na3 126.03(6) 8_544 2_455 ?
O2 P2 Na3 133.99(7) 8_545 2_455 ?
O6 P2 Na3 87.19(7) 2_556 2_455 ?
O2 P2 O8 140.93(14) . 2_455 ?
O5 P2 O8 85.53(14) 1_554 2_455 ?
O1 P2 O8 87.90(12) 2 2_455 ?
O4 P2 O8 37.77(13) . 2_455 ?
Na3 P2 O8 130.52(7) 8_544 2_455 ?
O2 P2 O8 93.33(8) 8_545 2_455 ?
O6 P2 O8 43.36(7) 2_556 2_455 ?
Na3 P2 O8 44.31(6) 2_455 2_455 ?
O7 P3 O8 113.27(18) . . ?
O7 P3 O6 113.53(17) . 1_654 ?
O8 P3 O6 113.21(17) . 1_654 ?
O7 P3 O4 103.43(16) . 2 ?
O8 P3 O4 105.30(19) . 2 ?
O6 P3 O4 107.04(16) 1_654 2 ?
O7 P3 Na2 44.81(11) . 5_654 ?
O8 P3 Na2 117.14(13) . 5_654 ?
O6 P3 Na2 129.65(12) 1_654 5_654 ?
O4 P3 Na2 59.03(11) 2 5_654 ?
O7 P3 O1 142.95(13) . 1_655 ?
O8 P3 O1 100.76(15) . 1_655 ?
O6 P3 O1 61.93(12) 1_654 1_655 ?
O4 P3 O1 51.41(11) 2 1_655 ?
Na2 P3 O1 106.80(6) 5_654 1_655 ?
O7 P3 Na3 106.82(13) . . ?
O8 P3 Na3 51.49(12) . . ?
O6 P3 Na3 139.29(12) 1_654 . ?
O4 P3 Na3 56.64(13) 2 . ?
Na2 P3 Na3 77.37(6) 5_654 . ?
O1 P3 Na3 82.70(6) 1_655 . ?
O7 P3 Na3 43.89(12) . 8_544 ?
O8 P3 Na3 70.48(14) . 8_544 ?
O6 P3 Na3 125.36(12) 1_654 8_544 ?
O4 P3 Na3 125.05(12) 2 8_544 ?
Na2 P3 Na3 74.27(4) 5_654 8_544 ?
O1 P3 Na3 170.00(7) 1_655 8_544 ?
Na3 P3 Na3 87.91(6) . 8_544 ?
O7 P3 Na3 88.63(12) . 1_554 ?
O8 P3 Na3 100.02(13) . 1_554 ?
O6 P3 Na3 38.79(12) 1_654 1_554 ?
O4 P3 Na3 144.47(12) 2 1_554 ?
Na2 P3 Na3 128.02(6) 5_654 1_554 ?
O1 P3 Na3 99.86(6) 1_655 1_554 ?
Na3 P3 Na3 150.95(7) . 1_554 ?
Na3 P3 Na3 86.69(5) 8_544 1_554 ?
O7 P3 Na2 35.10(12) . 1_654 ?
O8 P3 Na2 144.35(14) . 1_654 ?
O6 P3 Na2 81.77(12) 1_654 1_654 ?
O4 P3 Na2 100.17(13) 2 1_654 ?
Na2 P3 Na2 57.60(2) 5_654 1_654 ?
O1 P3 Na2 114.64(6) 1_655 1_654 ?
Na3 P3 Na2 134.46(6) . 1_654 ?
Na3 P3 Na2 74.56(4) 8_544 1_654 ?
Na3 P3 Na2 70.88(5) 1_554 1_654 ?
O7 P3 O7 66.21(9) . 8_545 ?
O8 P3 O7 77.46(13) . 8_545 ?
O6 P3 O7 166.89(13) 1_654 8_545 ?
O4 P3 O7 61.46(12) 2 8_545 ?
Na2 P3 O7 40.30(6) 5_654 8_545 ?
O1 P3 O7 109.74(7) 1_655 8_545 ?
Na3 P3 O7 41.49(6) . 8_545 ?
Na3 P3 O7 64.36(6) 8_544 8_545 ?
Na3 P3 O7 150.28(6) 1_554 8_545 ?
Na2 P3 O7 93.74(6) 1_654 8_545 ?
O7 P3 O1 113.88(13) . 6_655 ?
O8 P3 O1 58.34(13) . 6_655 ?
O6 P3 O1 60.43(12) 1_654 6_655 ?
O4 P3 O1 142.62(13) 2 6_655 ?
Na2 P3 O1 157.20(6) 5_654 6_655 ?
O1 P3 O1 95.93(9) 1_655 6_655 ?
Na3 P3 O1 107.83(6) . 6_655 ?
Na3 P3 O1 83.64(6) 8_544 6_655 ?
Na3 P3 O1 43.18(6) 1_554 6_655 ?
Na2 P3 O1 111.40(7) 1_654 6_655 ?
O7 P3 O1 132.40(7) 8_545 6_655 ?
O3 Na1 O3 140.60(8) 7_566 1_455 ?
O3 Na1 O3 140.60(8) 7_566 3_655 ?
O3 Na1 O3 56.95(12) 1_455 3_655 ?
O3 Na1 O3 56.95(12) 7_566 6_546 ?
O3 Na1 O3 140.60(8) 1_455 6_546 ?
O3 Na1 O3 140.60(8) 3_655 6_546 ?
O3 Na1 O5 56.17(8) 7_566 2_456 ?
O3 Na1 O5 88.09(8) 1_455 2_456 ?
O3 Na1 O5 103.91(8) 3_655 2_456 ?
O3 Na1 O5 110.47(8) 6_546 2_456 ?
O3 Na1 O5 110.47(8) 7_566 4_546 ?
O3 Na1 O5 103.91(8) 1_455 4_546 ?
O3 Na1 O5 88.09(8) 3_655 4_546 ?
O3 Na1 O5 56.17(8) 6_546 4_546 ?
O5 Na1 O5 166.47(11) 2_456 4_546 ?
O3 Na1 O5 103.91(8) 7_566 8_444 ?
O3 Na1 O5 56.17(8) 1_455 8_444 ?
O3 Na1 O5 110.47(8) 3_655 8_444 ?
O3 Na1 O5 88.09(8) 6_546 8_444 ?
O5 Na1 O5 90.795(18) 2_456 8_444 ?
O5 Na1 O5 90.795(19) 4_546 8_444 ?
O3 Na1 O5 88.09(8) 7_566 5_554 ?
O3 Na1 O5 110.47(8) 1_455 5_554 ?
O3 Na1 O5 56.17(8) 3_655 5_554 ?
O3 Na1 O5 103.91(8) 6_546 5_554 ?
O5 Na1 O5 90.795(19) 2_456 5_554 ?
O5 Na1 O5 90.795(18) 4_546 5_554 ?
O5 Na1 O5 166.47(11) 8_444 5_554 ?
O3 Na1 P1 151.53(6) 7_566 . ?
O3 Na1 P1 28.47(6) 1_455 . ?
O3 Na1 P1 28.47(6) 3_655 . ?
O3 Na1 P1 151.53(6) 6_546 . ?
O5 Na1 P1 96.76(5) 2_456 . ?
O5 Na1 P1 96.76(5) 4_546 . ?
O5 Na1 P1 83.24(5) 8_444 . ?
O5 Na1 P1 83.24(5) 5_554 . ?
O3 Na1 P1 28.47(6) 7_566 1_556 ?
O3 Na1 P1 151.53(6) 1_455 1_556 ?
O3 Na1 P1 151.53(6) 3_655 1_556 ?
O3 Na1 P1 28.47(6) 6_546 1_556 ?
O5 Na1 P1 83.24(5) 2_456 1_556 ?
O5 Na1 P1 83.24(5) 4_546 1_556 ?
O5 Na1 P1 96.76(5) 8_444 1_556 ?
O5 Na1 P1 96.76(5) 5_554 1_556 ?
P1 Na1 P1 180.0 . 1_556 ?
O3 Na1 O1 150.82(7) 7_566 3 ?
O3 Na1 O1 62.82(8) 1_455 3 ?
O3 Na1 O1 61.02(7) 3_655 3 ?
O3 Na1 O1 93.91(8) 6_546 3 ?
O5 Na1 O1 150.91(7) 2_456 3 ?
O5 Na1 O1 41.61(7) 4_546 3 ?
O5 Na1 O1 73.88(7) 8_444 3 ?
O5 Na1 O1 98.72(7) 5_554 3 ?
P1 Na1 O1 57.62(4) . 3 ?
P1 Na1 O1 122.38(4) 1_556 3 ?
O3 Na1 O1 61.02(7) 7_566 7_556 ?
O3 Na1 O1 150.82(7) 1_455 7_556 ?
O3 Na1 O1 93.91(8) 3_655 7_556 ?
O3 Na1 O1 62.82(8) 6_546 7_556 ?
O5 Na1 O1 98.72(7) 2_456 7_556 ?
O5 Na1 O1 73.88(7) 4_546 7_556 ?
O5 Na1 O1 150.91(7) 8_444 7_556 ?
O5 Na1 O1 41.61(7) 5_554 7_556 ?
P1 Na1 O1 122.38(4) . 7_556 ?
P1 Na1 O1 57.62(4) 1_556 7_556 ?
O1 Na1 O1 106.66(4) 3 7_556 ?
O7 Na2 O7 96.38(16) 3_666 1_456 ?
O7 Na2 O7 167.95(14) 3_666 8_445 ?
O7 Na2 O7 86.15(10) 1_456 8_445 ?
O7 Na2 O7 86.15(10) 3_666 5_565 ?
O7 Na2 O7 167.95(14) 1_456 5_565 ?
O7 Na2 O7 93.82(17) 8_445 5_565 ?
O7 Na2 O4 112.69(11) 3_666 6_556 ?
O7 Na2 O4 74.54(10) 1_456 6_556 ?
O7 Na2 O4 56.58(9) 8_445 6_556 ?
O7 Na2 O4 115.39(12) 5_565 6_556 ?
O7 Na2 O4 74.54(10) 3_666 7_566 ?
O7 Na2 O4 112.69(11) 1_456 7_566 ?
O7 Na2 O4 115.39(12) 8_445 7_566 ?
O7 Na2 O4 56.58(9) 5_565 7_566 ?
O4 Na2 O4 169.75(16) 6_556 7_566 ?
O7 Na2 Na2 48.19(8) 3_666 5 ?
O7 Na2 Na2 48.19(8) 1_456 5 ?
O7 Na2 Na2 133.09(8) 8_445 5 ?
O7 Na2 Na2 133.09(8) 5_565 5 ?
O4 Na2 Na2 95.13(8) 6_556 5 ?
O4 Na2 Na2 95.13(8) 7_566 5 ?
O7 Na2 Na2 131.81(8) 3_666 5_554 ?
O7 Na2 Na2 131.81(8) 1_456 5_554 ?
O7 Na2 Na2 46.91(8) 8_445 5_554 ?
O7 Na2 Na2 46.91(8) 5_565 5_554 ?
O4 Na2 Na2 84.87(8) 6_556 5_554 ?
O4 Na2 Na2 84.87(8) 7_566 5_554 ?
Na2 Na2 Na2 180.0 5 5_554 ?
O7 Na2 P3 143.02(8) 3_666 8_445 ?
O7 Na2 P3 77.23(8) 1_456 8_445 ?
O7 Na2 P3 26.40(7) 8_445 8_445 ?
O7 Na2 P3 107.68(11) 5_565 8_445 ?
O4 Na2 P3 30.35(6) 6_556 8_445 ?
O4 Na2 P3 141.77(10) 7_566 8_445 ?
Na2 Na2 P3 115.68(5) 5 8_445 ?
Na2 Na2 P3 64.32(5) 5_554 8_445 ?
O7 Na2 P3 77.23(8) 3_666 5_565 ?
O7 Na2 P3 143.02(8) 1_456 5_565 ?
O7 Na2 P3 107.68(11) 8_445 5_565 ?
O7 Na2 P3 26.40(7) 5_565 5_565 ?
O4 Na2 P3 141.77(10) 6_556 5_565 ?
O4 Na2 P3 30.35(6) 7_566 5_565 ?
Na2 Na2 P3 115.68(5) 5 5_565 ?
Na2 Na2 P3 64.32(5) 5_554 5_565 ?
P3 Na2 P3 128.65(9) 8_445 5_565 ?
O7 Na2 P3 21.73(7) 3_666 3_666 ?
O7 Na2 P3 102.93(10) 1_456 3_666 ?
O7 Na2 P3 146.28(7) 8_445 3_666 ?
O7 Na2 P3 83.73(7) 5_565 3_666 ?
O4 Na2 P3 94.16(7) 6_556 3_666 ?
O4 Na2 P3 91.26(7) 7_566 3_666 ?
Na2 Na2 P3 58.07(4) 5 3_666 ?
Na2 Na2 P3 121.93(4) 5_554 3_666 ?
P3 Na2 P3 123.58(3) 8_445 3_666 ?
P3 Na2 P3 84.56(3) 5_565 3_666 ?
O7 Na2 P3 102.93(10) 3_666 1_456 ?
O7 Na2 P3 21.73(7) 1_456 1_456 ?
O7 Na2 P3 83.73(7) 8_445 1_456 ?
O7 Na2 P3 146.28(7) 5_565 1_456 ?
O4 Na2 P3 91.26(7) 6_556 1_456 ?
O4 Na2 P3 94.16(7) 7_566 1_456 ?
Na2 Na2 P3 58.07(4) 5 1_456 ?
Na2 Na2 P3 121.93(4) 5_554 1_456 ?
P3 Na2 P3 84.56(3) 8_445 1_456 ?
P3 Na2 P3 123.58(3) 5_565 1_456 ?
P3 Na2 P3 116.15(8) 3_666 1_456 ?
O6 Na3 O7 97.70(12) 1_655 8_545 ?
O6 Na3 O1 78.41(11) 1_655 6_656 ?
O7 Na3 O1 132.96(13) 8_545 6_656 ?
O6 Na3 O5 67.69(11) 1_655 2_556 ?
O7 Na3 O5 115.28(11) 8_545 2_556 ?
O1 Na3 O5 106.46(11) 6_656 2_556 ?
O6 Na3 O8 160.64(13) 1_655 . ?
O7 Na3 O8 89.18(11) 8_545 . ?
O1 Na3 O8 109.89(11) 6_656 . ?
O5 Na3 O8 93.01(12) 2_556 . ?
O6 Na3 O4 108.72(12) 1_655 2 ?
O7 Na3 O4 73.81(10) 8_545 2 ?
O1 Na3 O4 152.23(12) 6_656 2 ?
O5 Na3 O4 55.86(9) 2_556 2 ?
O8 Na3 O4 55.84(10) . 2 ?
O6 Na3 P2 108.03(10) 1_655 8_545 ?
O7 Na3 P2 125.72(10) 8_545 8_545 ?
O1 Na3 P2 29.63(7) 6_656 8_545 ?
O5 Na3 P2 118.56(9) 2_556 8_545 ?
O8 Na3 P2 81.85(8) . 8_545 ?
O4 Na3 P2 134.66(10) 2 8_545 ?
O6 Na3 O8 103.73(11) 1_655 8_545 ?
O7 Na3 O8 52.69(10) 8_545 8_545 ?
O1 Na3 O8 82.33(10) 6_656 8_545 ?
O5 Na3 O8 165.43(11) 2_556 8_545 ?
O8 Na3 O8 94.85(10) . 8_545 ?
O4 Na3 O8 120.04(10) 2 8_545 ?
P2 Na3 O8 74.80(7) 8_545 8_545 ?
O6 Na3 O5 122.36(11) 1_655 8_544 ?
O7 Na3 O5 135.09(11) 8_545 8_544 ?
O1 Na3 O5 50.64(9) 6_656 8_544 ?
O5 Na3 O5 99.39(13) 2_556 8_544 ?
O8 Na3 O5 60.10(9) . 8_544 ?
O4 Na3 O5 107.26(10) 2 8_544 ?
P2 Na3 O5 28.30(6) 8_545 8_544 ?
O8 Na3 O5 95.17(10) 8_545 8_544 ?
O6 Na3 P3 138.46(10) 1_655 . ?
O7 Na3 P3 75.20(9) 8_545 . ?
O1 Na3 P3 136.05(9) 6_656 . ?
O5 Na3 P3 78.46(8) 2_556 . ?
O8 Na3 P3 27.22(7) . . ?
O4 Na3 P3 29.75(7) 2 . ?
P2 Na3 P3 109.00(6) 8_545 . ?
O8 Na3 P3 103.53(8) 8_545 . ?
O5 Na3 P3 85.42(7) 8_544 . ?
O6 Na3 P3 105.13(10) 1_655 8_545 ?
O7 Na3 P3 25.61(7) 8_545 8_545 ?
O1 Na3 P3 109.56(9) 6_656 8_545 ?
O5 Na3 P3 140.87(9) 2_556 8_545 ?
O8 Na3 P3 88.85(9) . 8_545 ?
O4 Na3 P3 94.73(8) 2 8_545 ?
P2 Na3 P3 100.41(6) 8_545 8_545 ?
O8 Na3 P3 27.46(6) 8_545 8_545 ?
O5 Na3 P3 115.06(8) 8_544 8_545 ?
P3 Na3 P3 86.04(5) . 8_545 ?
O6 Na3 P2 87.68(9) 1_655 2 ?
O7 Na3 P2 96.38(9) 8_545 2 ?
O1 Na3 P2 129.80(10) 6_656 2 ?
O5 Na3 P2 26.62(7) 2_556 2 ?
O8 Na3 P2 73.54(9) . 2 ?
O4 Na3 P2 29.27(6) 2 2 ?
P2 Na3 P2 130.68(7) 8_545 2 ?
O8 Na3 P2 147.77(8) 8_545 2 ?
O5 Na3 P2 104.02(8) 8_544 2 ?
P3 Na3 P2 53.62(4) . 2 ?
P3 Na3 P2 120.64(6) 8_545 2 ?
P2 O1 V1 128.94(17) 2_455 7_565 ?
P2 O1 O5 35.00(10) 2_455 2_456 ?
V1 O1 O5 152.85(15) 7_565 2_456 ?
P2 O1 Na3 94.60(14) 2_455 7_566 ?
V1 O1 Na3 129.84(13) 7_565 7_566 ?
O5 O1 Na3 77.16(11) 2_456 7_566 ?
P2 O1 O2 32.28(10) 2_455 2_455 ?
V1 O1 O2 119.40(14) 7_565 2_455 ?
O5 O1 O2 59.85(12) 2_456 2_455 ?
Na3 O1 O2 82.76(11) 7_566 2_455 ?
P2 O1 O4 36.35(10) 2_455 2_455 ?
V1 O1 O4 96.46(13) 7_565 2_455 ?
O5 O1 O4 59.23(11) 2_456 2_455 ?
Na3 O1 O4 130.82(13) 7_566 2_455 ?
O2 O1 O4 57.09(11) 2_455 2_455 ?
P2 O1 O2 94.07(14) 2_455 7_565 ?
V1 O1 O2 45.68(9) 7_565 7_565 ?
O5 O1 O2 129.07(14) 2_456 7_565 ?
Na3 O1 O2 119.94(13) 7_566 7_565 ?
O2 O1 O2 74.40(8) 2_455 7_565 ?
O4 O1 O2 78.30(12) 2_455 7_565 ?
P2 O1 O6 91.52(14) 2_455 1_554 ?
V1 O1 O6 44.83(8) 7_565 1_554 ?
O5 O1 O6 108.04(13) 2_456 1_554 ?
Na3 O1 O6 173.87(13) 7_566 1_554 ?
O2 O1 O6 102.58(13) 2_455 1_554 ?
O4 O1 O6 55.29(10) 2_455 1_554 ?
O2 O1 O6 59.56(10) 7_565 1_554 ?
P2 O1 O3 145.83(17) 2_455 7_565 ?
V1 O1 O3 42.47(8) 7_565 7_565 ?
O5 O1 O3 131.39(14) 2_456 7_565 ?
Na3 O1 O3 113.71(12) 7_566 7_565 ?
O2 O1 O3 160.70(15) 2_455 7_565 ?
O4 O1 O3 112.00(13) 2_455 7_565 ?
O2 O1 O3 88.13(12) 7_565 7_565 ?
O6 O1 O3 60.49(9) 1_554 7_565 ?
P2 O1 O8 146.98(17) 2_455 7_565 ?
V1 O1 O8 41.97(8) 7_565 7_565 ?
O5 O1 O8 165.15(15) 2_456 7_565 ?
Na3 O1 O8 88.19(11) 7_566 7_565 ?
O2 O1 O8 116.45(14) 2_455 7_565 ?
O4 O1 O8 132.77(14) 2_455 7_565 ?
O2 O1 O8 56.98(10) 7_565 7_565 ?
O6 O1 O8 86.73(11) 1_554 7_565 ?
O3 O1 O8 57.09(10) 7_565 7_565 ?
P2 O1 O6 142.61(17) 2_455 7_556 ?
V1 O1 O6 85.08(11) 7_565 7_556 ?
O5 O1 O6 119.05(13) 2_456 7_556 ?
Na3 O1 O6 48.03(8) 7_566 7_556 ?
O2 O1 O6 122.92(13) 2_455 7_556 ?
O4 O1 O6 178.18(14) 2_455 7_556 ?
O2 O1 O6 103.49(12) 7_565 7_556 ?
O6 O1 O6 125.84(11) 1_554 7_556 ?
O3 O1 O6 68.55(10) 7_565 7_556 ?
O8 O1 O6 49.03(9) 7_565 7_556 ?
P2 O1 P3 65.52(11) 2_455 1_455 ?
V1 O1 P3 72.70(8) 7_565 1_455 ?
O5 O1 P3 80.34(10) 2_456 1_455 ?
Na3 O1 P3 157.46(11) 7_566 1_455 ?
O2 O1 P3 84.85(10) 2_455 1_455 ?
O4 O1 P3 29.60(8) 2_455 1_455 ?
O2 O1 P3 74.16(9) 7_565 1_455 ?
O6 O1 P3 28.09(6) 1_554 1_455 ?
O3 O1 P3 82.49(9) 7_565 1_455 ?
O8 O1 P3 114.23(10) 7_565 1_455 ?
O6 O1 P3 151.03(11) 7_556 1_455 ?
P2 O2 V1 163.2(2) . . ?
P2 O2 O4 40.14(11) . . ?
V1 O2 O4 141.44(17) . . ?
P2 O2 O5 33.88(11) . 1_554 ?
V1 O2 O5 156.91(17) . 1_554 ?
O4 O2 O5 60.55(13) . 1_554 ?
P2 O2 O1 32.76(10) . 2 ?
V1 O2 O1 130.79(16) . 2 ?
O4 O2 O1 61.91(12) . 2 ?
O5 O2 O1 58.90(12) 1_554 2 ?
P2 O2 O1 143.67(19) . 6_655 ?
V1 O2 O1 48.45(9) . 6_655 ?
O4 O2 O1 146.78(15) . 6_655 ?
O5 O2 O1 110.21(14) 1_554 6_655 ?
O1 O2 O1 144.47(17) 2 6_655 ?
P2 O2 O8 119.95(18) . . ?
V1 O2 O8 47.49(9) . . ?
O4 O2 O8 146.12(16) . . ?
O5 O2 O8 121.61(16) 1_554 . ?
O1 O2 O8 89.49(13) 2 . ?
O1 O2 O8 67.00(11) 6_655 . ?
P2 O2 O6 142.18(18) . 6_656 ?
V1 O2 O6 46.45(9) . 6_656 ?
O4 O2 O6 102.21(14) . 6_656 ?
O5 O2 O6 138.95(15) 1_554 6_656 ?
O1 O2 O6 149.38(16) 2 6_656 ?
O1 O2 O6 62.44(11) 6_655 6_656 ?
O8 O2 O6 93.81(13) . 6_656 ?
P2 O2 O5 124.62(17) . 8_544 ?
V1 O2 O5 42.25(9) . 8_544 ?
O4 O2 O5 105.30(14) . 8_544 ?
O5 O2 O5 158.26(16) 1_554 8_544 ?
O1 O2 O5 100.45(13) 2 8_544 ?
O1 O2 O5 90.56(12) 6_655 8_544 ?
O8 O2 O5 59.87(11) . 8_544 ?
O6 O2 O5 56.37(10) 6_656 8_544 ?
P2 O2 O2 77.48(15) . 8_545 ?
V1 O2 O2 87.83(14) . 8_545 ?
O4 O2 O2 71.50(12) . 8_545 ?
O5 O2 O2 110.90(18) 1_554 8_545 ?
O1 O2 O2 55.56(11) 2 8_545 ?
O1 O2 O2 135.51(16) 6_655 8_545 ?
O8 O2 O2 77.45(10) . 8_545 ?
O6 O2 O2 95.51(13) 6_656 8_545 ?
O5 O2 O2 47.36(10) 8_544 8_545 ?
P2 O2 O2 96.54(18) . 8_544 ?
V1 O2 O2 98.00(15) . 8_544 ?
O4 O2 O2 104.34(14) . 8_544 ?
O5 O2 O2 63.09(12) 1_554 8_544 ?
O1 O2 O2 118.82(17) 2 8_544 ?
O1 O2 O2 50.05(10) 6_655 8_544 ?
O8 O2 O2 105.44(11) . 8_544 ?
O6 O2 O2 89.58(13) 6_656 8_544 ?
O5 O2 O2 138.65(17) 8_544 8_544 ?
O2 O2 O2 174.0(2) 8_545 8_544 ?
P2 O2 P2 122.98(17) . 8_544 ?
V1 O2 P2 72.54(10) . 8_544 ?
O4 O2 P2 119.82(13) . 8_544 ?
O5 O2 P2 89.99(12) 1_554 8_544 ?
O1 O2 P2 144.55(14) 2 8_544 ?
O1 O2 P2 28.04(7) 6_655 8_544 ?
O8 O2 P2 93.95(11) . 8_544 ?
O6 O2 P2 65.61(9) 6_656 8_544 ?
O5 O2 P2 111.74(11) 8_544 8_544 ?
O2 O2 P2 158.97(17) 8_545 8_544 ?
O2 O2 P2 27.00(7) 8_544 8_544 ?
P1 O3 V1 137.41(18) 1_655 . ?
P1 O3 O3 37.70(10) 1_655 3_755 ?
V1 O3 O3 167.4(2) . 3_755 ?
P1 O3 O3 34.02(5) 1_655 6_645 ?
V1 O3 O3 108.80(16) . 6_645 ?
O3 O3 O3 61.49(6) 3_755 6_645 ?
P1 O3 O3 34.02(5) 1_655 7_665 ?
V1 O3 O3 121.51(18) . 7_665 ?
O3 O3 O3 61.49(6) 3_755 7_665 ?
O3 O3 O3 57.02(13) 6_645 7_665 ?
P1 O3 Na1 99.23(12) 1_655 1_655 ?
V1 O3 Na1 121.13(13) . 1_655 ?
O3 O3 Na1 61.52(6) 3_755 1_655 ?
O3 O3 Na1 114.90(11) 6_645 1_655 ?
O3 O3 Na1 114.90(12) 7_665 1_655 ?
P1 O3 O5 158.40(17) 1_655 8_544 ?
V1 O3 O5 49.76(9) . 8_544 ?
O3 O3 O5 129.32(11) 3_755 8_544 ?
O3 O3 O5 131.51(15) 6_645 8_544 ?
O3 O3 O5 167.41(15) 7_665 8_544 ?
Na1 O3 O5 71.71(10) 1_655 8_544 ?
P1 O3 O8 137.86(16) 1_655 . ?
V1 O3 O8 46.17(9) . . ?
O3 O3 O8 146.41(18) 3_755 . ?
O3 O3 O8 138.86(17) 6_645 . ?
O3 O3 O8 103.94(14) 7_665 . ?
Na1 O3 O8 106.18(11) 1_655 . ?
O5 O3 O8 63.50(11) 8_544 . ?
P1 O3 O1 94.05(14) 1_655 6_655 ?
V1 O3 O1 45.48(8) . 6_655 ?
O3 O3 O1 131.72(8) 3_755 6_655 ?
O3 O3 O1 75.50(14) 6_645 6_655 ?
O3 O3 O1 77.61(15) 7_665 6_655 ?
Na1 O3 O1 166.55(13) 1_655 6_655 ?
O5 O3 O1 95.07(12) 8_544 6_655 ?
O8 O3 O1 64.30(10) . 6_655 ?
P1 O3 O6 110.08(14) 1_655 6_656 ?
V1 O3 O6 44.13(8) . 6_656 ?
O3 O3 O6 123.34(17) 3_755 6_656 ?
O3 O3 O6 76.09(12) 6_645 6_656 ?
O3 O3 O6 122.97(16) 7_665 6_656 ?
Na1 O3 O6 113.18(12) 1_655 6_656 ?
O5 O3 O6 59.13(11) 8_544 6_656 ?
O8 O3 O6 90.18(11) . 6_656 ?
O1 O3 O6 59.46(9) 6_655 6_656 ?
P1 O3 O1 77.53(11) 1_655 1_655 ?
V1 O3 O1 121.80(12) . 1_655 ?
O3 O3 O1 70.54(13) 3_755 1_655 ?
O3 O3 O1 110.30(11) 6_645 1_655 ?
O3 O3 O1 56.63(10) 7_665 1_655 ?
Na1 O3 O1 76.86(8) 1_655 1_655 ?
O5 O3 O1 117.69(12) 8_544 1_655 ?
O8 O3 O1 76.29(10) . 1_655 ?
O1 O3 O1 108.37(9) 6_655 1_655 ?
O6 O3 O1 165.26(12) 6_656 1_655 ?
P1 O3 O6 90.45(12) 1_655 1_654 ?
V1 O3 O6 79.31(10) . 1_654 ?
O3 O3 O6 110.08(14) 3_755 1_654 ?
O3 O3 O6 104.10(14) 6_645 1_654 ?
O3 O3 O6 56.45(11) 7_665 1_654 ?
Na1 O3 O6 122.89(11) 1_655 1_654 ?
O5 O3 O6 111.01(12) 8_544 1_654 ?
O8 O3 O6 47.51(9) . 1_654 ?
O1 O3 O6 58.74(9) 6_655 1_654 ?
O6 O3 O6 115.61(9) 6_656 1_654 ?
O1 O3 O6 50.52(8) 1_655 1_654 ?
P2 O4 P3 131.8(2) . 2_455 ?
P2 O4 O2 36.70(10) . . ?
P3 O4 O2 150.82(19) 2_455 . ?
P2 O4 O7 161.55(19) . 2_455 ?
P3 O4 O7 36.64(9) 2_455 2_455 ?
O2 O4 O7 141.12(18) . 2_455 ?
P2 O4 O5 35.79(10) . 1_554 ?
P3 O4 O5 129.2(2) 2_455 1_554 ?
O2 O4 O5 61.06(12) . 1_554 ?
O7 O4 O5 157.38(18) 2_455 1_554 ?
P2 O4 O8 118.89(18) . 2_455 ?
P3 O4 O8 35.95(11) 2_455 2_455 ?
O2 O4 O8 155.57(17) . 2_455 ?
O7 O4 O8 61.37(13) 2_455 2_455 ?
O5 O4 O8 98.00(16) 1_554 2_455 ?
P2 O4 O6 101.98(15) . 2_556 ?
P3 O4 O6 35.21(9) 2_455 2_556 ?
O2 O4 O6 116.18(15) . 2_556 ?
O7 O4 O6 61.13(11) 2_455 2_556 ?
O5 O4 O6 118.95(15) 1_554 2_556 ?
O8 O4 O6 60.77(11) 2_455 2_556 ?
P2 O4 O1 33.83(9) . 2 ?
P3 O4 O1 98.99(15) 2_455 2 ?
O2 O4 O1 61.01(11) . 2 ?
O7 O4 O1 129.18(15) 2_455 2 ?
O5 O4 O1 58.77(11) 1_554 2 ?
O8 O4 O1 98.25(13) 2_455 2 ?
O6 O4 O1 68.28(11) 2_556 2 ?
P2 O4 Na3 95.11(15) . 2_455 ?
P3 O4 Na3 93.60(15) 2_455 2_455 ?
O2 O4 Na3 112.25(13) . 2_455 ?
O7 O4 Na3 99.72(13) 2_455 2_455 ?
O5 O4 Na3 59.36(11) 1_554 2_455 ?
O8 O4 Na3 59.50(11) 2_455 2_455 ?
O6 O4 Na3 118.78(14) 2_556 2_455 ?
O1 O4 Na3 108.42(13) 2 2_455 ?
P2 O4 Na2 135.34(17) . 6_656 ?
P3 O4 Na2 90.62(12) 2_455 6_656 ?
O2 O4 Na2 99.90(13) . 6_656 ?
O7 O4 Na2 54.24(9) 2_455 6_656 ?
O5 O4 Na2 130.39(15) 1_554 6_656 ?
O8 O4 Na2 103.66(12) 2_455 6_656 ?
O6 O4 Na2 110.59(13) 2_556 6_656 ?
O1 O4 Na2 153.81(15) 2 6_656 ?
Na3 O4 Na2 95.10(10) 2_455 6_656 ?
P2 O4 O7 128.46(16) . 7_565 ?
P3 O4 O7 91.19(13) 2_455 7_565 ?
O2 O4 O7 115.82(14) . 7_565 ?
O7 O4 O7 69.97(7) 2_455 7_565 ?
O5 O4 O7 97.77(13) 1_554 7_565 ?
O8 O4 O7 77.23(12) 2_455 7_565 ?
O6 O4 O7 126.11(13) 2_556 7_565 ?
O1 O4 O7 155.63(15) 2 7_565 ?
Na3 O4 O7 48.49(8) 2_455 7_565 ?
Na2 O4 O7 46.67(8) 6_656 7_565 ?
P2 O4 O2 71.41(13) . 8_545 ?
P3 O4 O2 86.34(13) 2_455 8_545 ?
O2 O4 O2 64.78(9) . 8_545 ?
O7 O4 O2 91.50(12) 2_455 8_545 ?
O5 O4 O2 106.59(12) 1_554 8_545 ?
O8 O4 O2 114.76(13) 2_455 8_545 ?
O6 O4 O2 54.33(10) 2_556 8_545 ?
O1 O4 O2 53.12(10) 2 8_545 ?
Na3 O4 O2 161.10(13) 2_455 8_545 ?
Na2 O4 O2 103.80(12) 6_656 8_545 ?
O7 O4 O2 150.39(13) 7_565 8_545 ?
P2 O5 V1 140.4(2) 1_556 8_545 ?
P2 O5 O1 35.07(10) 1_556 2_556 ?
V1 O5 O1 146.84(16) 8_545 2_556 ?
P2 O5 O4 38.57(11) 1_556 1_556 ?
V1 O5 O4 141.62(16) 8_545 1_556 ?
O1 O5 O4 62.01(11) 2_556 1_556 ?
P2 O5 O2 33.44(10) 1_556 1_556 ?
V1 O5 O2 107.01(15) 8_545 1_556 ?
O1 O5 O2 61.25(11) 2_556 1_556 ?
O4 O5 O2 58.39(12) 1_556 1_556 ?
P2 O5 Na3 103.30(16) 1_556 2_456 ?
V1 O5 Na3 97.67(12) 8_545 2_456 ?
O1 O5 Na3 115.47(14) 2_556 2_456 ?
O4 O5 Na3 64.78(11) 1_556 2_456 ?
O2 O5 Na3 114.61(14) 1_556 2_456 ?
P2 O5 O3 161.85(19) 1_556 8_545 ?
V1 O5 O3 45.95(8) 8_545 8_545 ?
O1 O5 O3 127.88(15) 2_556 8_545 ?
O4 O5 O3 153.70(16) 1_556 8_545 ?
O2 O5 O3 147.12(16) 1_556 8_545 ?
Na3 O5 O3 90.67(11) 2_456 8_545 ?
P2 O5 O6 133.97(18) 1_556 2_556 ?
V1 O5 O6 46.72(8) 8_545 2_556 ?
O1 O5 O6 165.31(16) 2_556 2_556 ?
O4 O5 O6 103.49(14) 1_556 2_556 ?
O2 O5 O6 114.53(15) 1_556 2_556 ?
Na3 O5 O6 51.88(9) 2_456 2_556 ?
O3 O5 O6 64.02(10) 8_545 2_556 ?
P2 O5 O8 110.76(17) 1_556 8_545 ?
V1 O5 O8 44.59(9) 8_545 8_545 ?
O1 O5 O8 102.31(14) 2_556 8_545 ?
O4 O5 O8 145.52(16) 1_556 8_545 ?
O2 O5 O8 87.15(13) 1_556 8_545 ?
Na3 O5 O8 141.89(14) 2_456 8_545 ?
O3 O5 O8 60.56(11) 8_545 8_545 ?
O6 O5 O8 91.22(12) 2_556 8_545 ?
P2 O5 O2 102.53(15) 1_556 8_545 ?
V1 O5 O2 39.72(8) 8_545 8_545 ?
O1 O5 O2 127.02(14) 2_556 8_545 ?
O4 O5 O2 107.46(14) 1_556 8_545 ?
O2 O5 O2 69.55(8) 1_556 8_545 ?
Na3 O5 O2 101.48(12) 2_456 8_545 ?
O3 O5 O2 85.65(12) 8_545 8_545 ?
O6 O5 O2 57.06(10) 2_556 8_545 ?
O8 O5 O2 55.37(10) 8_545 8_545 ?
P2 O5 Na1 116.04(15) 1_556 2_556 ?
V1 O5 Na1 97.84(10) 8_545 2_556 ?
O1 O5 Na1 83.05(11) 2_556 2_556 ?
O4 O5 Na1 114.26(13) 1_556 2_556 ?
O2 O5 Na1 143.12(14) 1_556 2_556 ?
Na3 O5 Na1 87.81(9) 2_456 2_556 ?
O3 O5 Na1 52.12(8) 8_545 2_556 ?
O6 O5 Na1 102.35(11) 2_556 2_556 ?
O8 O5 Na1 92.12(11) 8_545 2_556 ?
O2 O5 Na1 137.09(11) 8_545 2_556 ?
P2 O5 Na3 73.22(13) 1_556 8_545 ?
V1 O5 Na3 95.20(11) 8_545 8_545 ?
O1 O5 Na3 52.21(9) 2_556 8_545 ?
O4 O5 Na3 110.58(12) 1_556 8_545 ?
O2 O5 Na3 72.15(11) 1_556 8_545 ?
Na3 O5 Na3 162.68(13) 2_456 8_545 ?
O3 O5 Na3 89.98(11) 8_545 8_545 ?
O6 O5 Na3 141.92(13) 2_556 8_545 ?
O8 O5 Na3 50.85(9) 8_545 8_545 ?
O2 O5 Na3 95.83(11) 8_545 8_545 ?
Na1 O5 Na3 78.96(8) 2_556 8_545 ?
P3 O6 V1 135.18(18) 1_456 7_566 ?
P3 O6 Na3 117.16(16) 1_456 1_455 ?
V1 O6 Na3 107.54(13) 7_566 1_455 ?
P3 O6 O4 37.75(10) 1_456 2_456 ?
V1 O6 O4 98.49(12) 7_566 2_456 ?
Na3 O6 O4 153.30(15) 1_455 2_456 ?
P3 O6 O7 32.99(10) 1_456 1_456 ?
V1 O6 O7 147.44(15) 7_566 1_456 ?
Na3 O6 O7 95.76(13) 1_455 1_456 ?
O4 O6 O7 57.97(11) 2_456 1_456 ?
P3 O6 O8 33.33(10) 1_456 1_456 ?
V1 O6 O8 130.70(15) 7_566 1_456 ?
Na3 O6 O8 105.57(14) 1_455 1_456 ?
O4 O6 O8 58.98(12) 2_456 1_456 ?
O7 O6 O8 59.69(12) 1_456 1_456 ?
P3 O6 O5 173.19(18) 1_456 2_456 ?
V1 O6 O5 48.20(9) 7_566 2_456 ?
Na3 O6 O5 60.43(10) 1_455 2_456 ?
O4 O6 O5 142.93(15) 2_456 2_456 ?
O7 O6 O5 140.35(15) 1_456 2_456 ?
O8 O6 O5 151.95(15) 1_456 2_456 ?
P3 O6 O2 111.29(16) 1_456 7_566 ?
V1 O6 O2 44.86(9) 7_566 7_566 ?
Na3 O6 O2 116.74(13) 1_455 7_566 ?
O4 O6 O2 78.01(12) 2_456 7_566 ?
O7 O6 O2 104.38(13) 1_456 7_566 ?
O8 O6 O2 136.45(14) 1_456 7_566 ?
O5 O6 O2 66.56(11) 2_456 7_566 ?
P3 O6 O1 89.98(14) 1_456 1_556 ?
V1 O6 O1 45.86(8) 7_566 1_556 ?
Na3 O6 O1 150.01(14) 1_455 1_556 ?
O4 O6 O1 56.43(10) 2_456 1_556 ?
O7 O6 O1 114.23(13) 1_456 1_556 ?
O8 O6 O1 90.03(12) 1_456 1_556 ?
O5 O6 O1 93.99(12) 2_456 1_556 ?
O2 O6 O1 58.00(10) 7_566 1_556 ?
P3 O6 O3 129.94(17) 1_456 7_566 ?
V1 O6 O3 42.17(7) 7_566 7_566 ?
Na3 O6 O3 91.18(12) 1_455 7_566 ?
O4 O6 O3 112.63(13) 2_456 7_566 ?
O7 O6 O3 162.10(15) 1_456 7_566 ?
O8 O6 O3 102.55(13) 1_456 7_566 ?
O5 O6 O3 56.85(10) 2_456 7_566 ?
O2 O6 O3 87.01(11) 7_566 7_566 ?
O1 O6 O3 60.05(9) 1_556 7_566 ?
P3 O6 O1 94.15(14) 1_456 6_556 ?
V1 O6 O1 110.40(12) 7_566 6_556 ?
Na3 O6 O1 53.55(9) 1_455 6_556 ?
O4 O6 O1 122.31(14) 2_456 6_556 ?
O7 O6 O1 101.67(12) 1_456 6_556 ?
O8 O6 O1 64.36(11) 1_456 6_556 ?
O5 O6 O1 89.11(11) 2_456 6_556 ?
O2 O6 O1 153.16(14) 7_566 6_556 ?
O1 O6 O1 115.86(14) 1_556 6_556 ?
O3 O6 O1 69.50(10) 7_566 6_556 ?
P3 O6 P2 64.43(11) 1_456 2_456 ?
V1 O6 P2 70.78(8) 7_566 2_456 ?
Na3 O6 P2 177.32(13) 1_455 2_456 ?
O4 O6 P2 28.88(7) 2_456 2_456 ?
O7 O6 P2 86.62(11) 1_456 2_456 ?
O8 O6 P2 74.55(10) 1_456 2_456 ?
O5 O6 P2 118.25(12) 2_456 2_456 ?
O2 O6 P2 63.68(9) 7_566 2_456 ?
O1 O6 P2 27.62(6) 1_556 2_456 ?
O3 O6 P2 86.19(9) 7_566 2_456 ?
O1 O6 P2 124.77(11) 6_556 2_456 ?
P3 O7 Na2 123.17(17) . 1_654 ?
P3 O7 Na2 108.78(15) . 5_654 ?
Na2 O7 Na2 84.90(9) 1_654 5_654 ?
P3 O7 Na3 110.50(16) . 8_544 ?
Na2 O7 Na3 116.40(13) 1_654 8_544 ?
Na2 O7 Na3 108.84(12) 5_654 8_544 ?
P3 O7 O4 39.94(11) . 2 ?
Na2 O7 O4 114.00(14) 1_654 2 ?
Na2 O7 O4 69.18(10) 5_654 2 ?
Na3 O7 O4 129.16(16) 8_544 2 ?
P3 O7 O8 33.54(10) . . ?
Na2 O7 O8 152.20(15) 1_654 . ?
Na2 O7 O8 114.23(15) 5_654 . ?
Na3 O7 O8 77.82(12) 8_544 . ?
O4 O7 O8 60.14(14) 2 . ?
P3 O7 O6 33.48(10) . 1_654 ?
Na2 O7 O6 92.57(12) 1_654 1_654 ?
Na2 O7 O6 123.74(14) 5_654 1_654 ?
Na3 O7 O6 121.92(14) 8_544 1_654 ?
O4 O7 O6 60.90(12) 2 1_654 ?
O8 O7 O6 60.29(11) . 1_654 ?
P3 O7 O4 145.50(17) . 6_655 ?
Na2 O7 O4 58.78(9) 1_654 6_655 ?
Na2 O7 O4 105.70(11) 5_654 6_655 ?
Na3 O7 O4 57.70(10) 8_544 6_655 ?
O4 O7 O4 172.08(19) 2 6_655 ?
O8 O7 O4 127.71(14) . 6_655 ?
O6 O7 O4 120.50(13) 1_654 6_655 ?
P3 O7 O7 88.51(14) . 8_545 ?
Na2 O7 O7 129.99(9) 1_654 8_545 ?
Na2 O7 O7 46.30(8) 5_654 8_545 ?
Na3 O7 O7 78.43(11) 8_544 8_545 ?
O4 O7 O7 64.41(11) 2 8_545 ?
O8 O7 O7 74.40(10) . 8_545 ?
O6 O7 O7 120.84(15) 1_654 8_545 ?
O4 O7 O7 116.86(15) 6_655 8_545 ?
P3 O7 O7 106.90(15) . 8_544 ?
Na2 O7 O7 47.55(8) 1_654 8_544 ?
Na2 O7 O7 131.25(9) 5_654 8_544 ?
Na3 O7 O7 88.06(12) 8_544 8_544 ?
O4 O7 O7 133.09(16) 2 8_544 ?
O8 O7 O7 113.94(11) . 8_544 ?
O6 O7 O7 75.90(11) 1_654 8_544 ?
O4 O7 O7 45.61(10) 6_655 8_544 ?
O7 O7 O7 162.4(2) 8_545 8_544 ?
P3 O7 O7 126.21(19) . 3_765 ?
Na2 O7 O7 41.81(8) 1_654 3_765 ?
Na2 O7 O7 43.09(8) 5_654 3_765 ?
Na3 O7 O7 121.41(15) 8_544 3_765 ?
O4 O7 O7 92.35(13) 2 3_765 ?
O8 O7 O7 151.82(14) . 3_765 ?
O6 O7 O7 113.74(14) 1_654 3_765 ?
O4 O7 O7 79.96(11) 6_655 3_765 ?
O7 O7 O7 88.76(3) 8_545 3_765 ?
O7 O7 O7 88.76(3) 8_544 3_765 ?
P3 O7 O8 103.01(14) . 8_544 ?
Na2 O7 O8 87.05(11) 1_654 8_544 ?
Na2 O7 O8 146.30(12) 5_654 8_544 ?
Na3 O7 O8 47.54(9) 8_544 8_544 ?
O4 O7 O8 142.82(14) 2 8_544 ?
O8 O7 O8 86.68(13) . 8_544 ?
O6 O7 O8 89.24(12) 1_654 8_544 ?
O4 O7 O8 43.72(9) 6_655 8_544 ?
O7 O7 O8 125.60(11) 8_545 8_544 ?
O7 O7 O8 43.69(8) 8_544 8_544 ?
O7 O7 O8 121.43(10) 3_765 8_544 ?
P3 O8 V1 134.71(19) . . ?
P3 O8 O4 38.74(11) . 2 ?
V1 O8 O4 141.96(17) . 2 ?
P3 O8 O7 33.19(10) . . ?
V1 O8 O7 144.39(18) . . ?
O4 O8 O7 58.49(12) 2 . ?
P3 O8 O6 33.47(10) . 1_654 ?
V1 O8 O6 101.36(13) . 1_654 ?
O4 O8 O6 60.26(12) 2 1_654 ?
O7 O8 O6 60.02(12) . 1_654 ?
P3 O8 Na3 101.29(15) . . ?
V1 O8 Na3 113.98(14) . . ?
O4 O8 Na3 64.66(11) 2 . ?
O7 O8 Na3 101.32(13) . . ?
O6 O8 Na3 123.29(14) 1_654 . ?
P3 O8 O2 136.4(2) . . ?
V1 O8 O2 45.13(9) . . ?
O4 O8 O2 172.39(17) 2 . ?
O7 O8 O2 114.21(16) . . ?
O6 O8 O2 119.21(15) 1_654 . ?
Na3 O8 O2 117.20(14) . . ?
P3 O8 O3 105.86(16) . . ?
V1 O8 O3 43.40(9) . . ?
O4 O8 O3 98.58(13) 2 . ?
O7 O8 O3 137.25(14) . . ?
O6 O8 O3 77.38(12) 1_654 . ?
Na3 O8 O3 98.91(13) . . ?
O2 O8 O3 88.50(12) . . ?
P3 O8 O5 155.4(2) . 8_544 ?
V1 O8 O5 45.25(9) . 8_544 ?
O4 O8 O5 121.69(15) 2 8_544 ?
O7 O8 O5 166.21(15) . 8_544 ?
O6 O8 O5 133.31(15) 1_654 8_544 ?
Na3 O8 O5 69.05(11) . 8_544 ?
O2 O8 O5 64.76(11) . 8_544 ?
O3 O8 O5 55.94(10) . 8_544 ?
P3 O8 O1 96.44(15) . 6_655 ?
V1 O8 O1 42.26(8) . 6_655 ?
O4 O8 O1 125.77(14) 2 6_655 ?
O7 O8 O1 103.37(14) . 6_655 ?
O6 O8 O1 66.61(11) 1_654 6_655 ?
Na3 O8 O1 154.74(15) . 6_655 ?
O2 O8 O1 56.02(10) . 6_655 ?
O3 O8 O1 58.61(10) . 6_655 ?
O5 O8 O1 87.46(11) 8_544 6_655 ?
P3 O8 Na3 82.06(14) . 8_544 ?
V1 O8 Na3 113.37(13) . 8_544 ?
O4 O8 Na3 102.93(12) 2 8_544 ?
O7 O8 Na3 49.49(10) . 8_544 ?
O6 O8 Na3 99.59(13) 1_654 8_544 ?
Na3 O8 Na3 104.67(11) . 8_544 ?
O2 O8 Na3 69.50(11) . 8_544 ?
O3 O8 Na3 153.17(13) . 8_544 ?
O5 O8 Na3 121.85(12) 8_544 8_544 ?
O1 O8 Na3 95.44(12) 6_655 8_544 ?
P3 O8 O7 77.64(13) . 8_545 ?
V1 O8 O7 147.60(14) . 8_545 ?
O4 O8 O7 59.05(10) 2 8_545 ?
O7 O8 O7 61.91(8) . 8_545 ?
O6 O8 O7 110.78(13) 1_654 8_545 ?
Na3 O8 O7 43.28(8) . 8_545 ?
O2 O8 O7 116.59(13) . 8_545 ?
O3 O8 O7 140.41(13) . 8_545 ?
O5 O8 O7 105.55(12) 8_544 8_545 ?
O1 O8 O7 160.89(14) 6_655 8_545 ?
Na3 O8 O7 65.90(8) 8_544 8_545 ?
 
_refine_diff_density_max    0.523
_refine_diff_density_min   -0.442
_refine_diff_density_rms    0.117
